3D and Planar Constitutive Relations


 Allison Ashlee Hensley
 1 years ago
 Views:
Transcription
1 3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace Engineering Indian Institute of Technology Kanpur 5 January 017
2 3D Constitutive Relations
3 Generalized Hooke s Law: Generalized Hooke s law of the proportionality of stress and strain: Each of the six component of the stress at any point is a linear function of the six components of strain at that point. Concept of initial state Loading under two situations:  Isothermal and Reversible;  Adiabatic and Reversible. Stress components are the partial differential coefficients of a function (W) of the straincomponents. 1 W W σ ij = + ε ij ε ji
4 Generalized Hooke s Law: Form of the Strain Energy Density Function (W): Homogeneous quadratic function of the strain components. 1 W = constant + C ij ε ij + C ijkl ε ij ε kl W is invariant Cij and Cijkl are tensors. W is taken to be zero when body is in the initial state in which Then, constant is zero. ε ij are zero.
5 Generalized Hooke s Law: For unstrained and unstressed body, Cij are zero. This leads to 1 W = Cijkl ε ij ε kl and σ ij = C ijkl ε kl i, j, k, l = 1,, 3 Cijkl is a fourth order (stiffness) tensor/matrix. (3 ) 4 = 81 independent constants!
6 Generalized Hooke s Law: Simply, you can view this as if you have a vector of 9 stress components which is related to a vector of 9 strain components through a matrix of 9x9! {σ }9 1 = [C ]9 9 {ε }9 1 C1111 C111 C1311 C111 [C] = C11 C311 C 3111 C311 C3311 C111 C1113 C111 C11 C113 C1131 C113 C1133 C11 C113 C11 C1 C13 C131 C13 C133 C131 C1313 C131 C13 C133 C1331 C133 C1333 C11 C113 C11 C1 C13 C131 C13 C133 C1 C13 C1 C C3 C31 C3 C33 C31 C313 C31 C3 C33 C331 C33 C333 C311 C3113 C311 C31 C313 C3131 C313 C3133 C31 C313 C31 C3 C33 C331 C33 C333 C331 C3313 C331 C33 C333 C3331 C333 C3333
7 Stress Tensor Symmetry: Stress symmetry: σ ij = σ ji σ ij = C ijkl ε kl σ ji = C jikl ε kl σ ij σ ji = 0 ( Cijkl C jikl ) ε kl = 0 C ijkl = C jikl six independent ways to express when i and j are taken together and still 9 ways to express k and l taken together. 6 9 = 54 independent constants!
8 Stress Tensor Symmetry: Simply, you can view this as if you have a vector of 6 stress components which is related to a vector of 9 strain components through a matrix of 6x9! {σ }6 1 = [C ]6 9 {ε }9 1 C1111 C 11 C3311 [C] = C 311 C 1311 C111 C111 C1 C331 C31 C1113 C13 C3313 C313 C111 C1 C331 C31 C11 C C33 C3 C113 C3 C333 C33 C1131 C31 C3331 C331 C113 C3 C333 C33 C131 C1313 C131 C13 C133 C1331 C133 C11 C113 C11 C1 C13 C131 C13 C1133 C33 C3333 C333 C1333 C133
9 Stress and Strain Tensor Symmetry: Strain symmetry: ε ij = ε ji σ ij = C ijkl ε kl σ ij = C ijlk ε lk σ ij σ ij = 0 ( Cijkl Cijlk ) ε kl = 0 C ijkl = C ijlk six independent ways to express when i and j are taken together and 6 ways to express k and l taken together. 6 6 = 36 independent constants!
10 Stress and Strain Tensor Symmetry: Or simply, you can view this as if you have a vector of 6 stress components which is related to a vector of 6 strain components through a matrix of 6x6! {σ }6 1 = [C ]6 6 {ε }6 1 C1111 C 11 C3311 [C] = C 311 C 1311 C111 C11 C C33 C3 C1133 C33 C3333 C333 C113 C3 C333 C33 C1113 C13 C3313 C31 C13 C1333 C133 C1313 C1 C133 C13 C11 C111 C1 C331 C31 C131 C11
11 Stress and Strain Tensor Symmetry: In other words, σ11 C1111 σ C 11 σ33 C3311 = σ3 C311 σ13 C1311 σ1 C111 C11 C1133 C113 C1113 C111 ε11 C C33 C3 C13 C1 ε C33 C3333 C333 C3313 C331 ε33 C3 C333 C33 C31 C31 ε3 C13 C1333 C133 C1313 C131 ε13 C1 C133 C13 C11 C11 ε1
12 Voigt Notation: Using Voigt notation  a way to represent a symmetric tensor by reducing its order For stress components: {σ σ11 σ1 σ13 1 σ σ 3 4 σ33 3 σ σ33 σ3 σ13 σ1} ={σ1 σ σ3 σ4 σ5 σ6} Strain Components: {ε11 ε ε33 ε3 ε13 ε1} ={ε1 ε ε3 ε4 ε5 ε6}
13 Stress and Strain Tensor Symmetries: Instead of writing C as a fourth order tensor, written as a second order tensor and stress and strains tensors are written as vectors! σ1 C11 σ C 1 σ3 C31 = σ4 C41 σ5 C51 σ6 C61 C1 C13 C14 C15 C16 ε1 C C3 C4 C5 C6 ε C3 C33 C34 C35 C36 ε3 C4 C43 C44 C45 C46 ε4 C51 C53 C54 C55 C56 ε5 C6 C63 C64 C65 C66 ε6
14 Existence of W: Existence of W : Hyperelastic materials Invariant Positive Definite 1 W = C ij ε j ε i 1 W = C ij ε i ε j ( Cij C ji ) ε iε j = 0 C ij = C ji
15 Existence of W: σ1 C11 C1 C13 σ C C 3 σ3 C33 = σ4 σ5 σ6 C14 C15 C16 ε1 C4 C5 C6 ε C34 C35 C36 ε3 C44 C45 C46 ε4 C55 C56 ε5 C66 ε6 1 independent constants!
16 Symmetries: Stress symmetry C ijkl = C jikl Minor Symmetries Strain symmetry C ijkl = C jikl Existence of W: C ijkl = C klij Major Symmetry
17 Transformations: Transformations Prime denotes the transformed coordinates. aij denotes the components of a transformation matrix
18 Material Symmetry: Further reduction in constants obtained by material symmetry Symmetry Definition: Any geometrical figure which can be brought to coincidence with itself, by an operation which changes the position of any of its points, is said to possess symmetry. Rotation and Reflection
19 Form of W: Quadratic in strain components: Note that the strains used are engineering strains.
20 Material Symmetry: One Plane of Material Symmetry: Monoclinic Materials
21 Material Symmetry: One Plane of Material Symmetry Transformation of axes: Transformation matrix: Transformation of strains:
22 Material Symmetry: One Plane of Material Symmetry Transformation of stresses:
23 Material Symmetry: One Plane of Material Symmetry Transformation of stiffness: C ij' = C ij Comparison of stress components: C14 = C15 = 0
24 Material Symmetry: One Plane of Material Symmetry Similarly, 13 independent constants
25 Material Symmetry: One Plane of Material Symmetry Second Approach: Invariance of W W for Hyperelastic material
26 Material Symmetry: One Plane of Material Symmetry Second Approach: Invariance of W For W to be invariant the product terms ε 1ε 4, ε 1ε 5, ε ε 4, ε ε 5, ε 3ε 4, ε 3ε 5, ε 4 ε 6, ε 5ε 6 must vanish, that is, C14, C15, C 4, C 5, C 34, C 35, C 46, C 56 are zero
27 Material Symmetry: Two Orthogonal Planes of Material Symmetry Two Orthogonal Planes of Material Symmetry: Orthotropic Materials Transformation of axes: Transformation matrix: Transformation of strains:
28 Material Symmetry: Two Orthogonal Planes of Material Symmetry Transformation of stresses: Transformation of stiffness: C ij' = C ij
29 Material Symmetry: Two Orthogonal Planes of Material Symmetry Comparison of stresses: C16 = 0 Similarly,
30 Material Symmetry: Two Orthogonal Planes of Material Symmetry Stiffness Tensor: 9 independent constants
31 Material Symmetry: Two Orthogonal Planes of Material Symmetry Second approach: Invariance of w W for monoclinic material: C11ε 1 + C ε + C33ε 3 + C 44 ε C55ε 5 + C 66ε 6 + C1ε 1ε + C13ε 1ε 3 + W = C16ε 1ε 6 + C 3ε ε 3 + C 6 ε ε 6 + C36ε 3ε 6 C 45ε 4 ε 5 or form of W: ε 1, ε, ε 3, ε 4, ε 5, ε 6, W = W ε 1ε, ε 1ε 3, ε 1ε 6, ε ε, ε ε, ε ε, ε ε
32 Material Symmetry: Two Orthogonal Planes of Material Symmetry For W to be invariant under the strain transformations the product terms ε 1ε 6, ε ε 6, ε 3ε 6, ε 4 ε 5 must vanish, which is possible when C16, C 6, C36, C 45 are zero W for orthotropic material: 1 C11ε 1 + C ε + C33ε 3 + C 44 ε 4 + C55ε 5 + C 66ε 6 W = C1 ε 1ε + C13ε 1ε 3 + C 3ε ε 3 +
33 Material Symmetry: Two Orthogonal Planes of Material Symmetry When material has two orthogonal planes of symmetry then it also symmetric about a plane which is mutually orthogonal earlier two planes! Such materials are called Orthotropic Materials. Select now the remaining plane x1x3 as the third orthogonal plane of material symmetry in addition to earlier two planes Follow the same procedure, either comparing the stresses or invariance of W There will be no change in the final stiffness tensor. Number of independent constants will be still 9!
34 Material Symmetry: Two Orthogonal Planes of Material Symmetry When material has two orthogonal planes of symmetry then it also symmetric about a plane which is mutually orthogonal earlier two planes! Alternately: Now select the plane x1x3 as the second orthogonal plane of material symmetry in addition to x1x plane
35 Isotropy in a Plane: Isotropic behaviour of UD lamina in the crosssectional plane (perpendicular to fibre s length) Transformation matrix:
36 Isotropy in a Plane: Transformation of strains:
37 Material Symmetry: Two Orthogonal Planes of Material Symmetry W for monoclinic material: ε 1, ε, ε 3, ε 4, ε 5, ε 6, W = W ε 1ε, ε 1ε 3, ε 1ε 6, ε ε, ε ε, ε ε, ε ε For invariance ε 1ε 6, ε ε 6, ε 3ε 6, ε 4 ε 5 = 0 C16, C 6, C 36, C 45 are zero
38 Isotropy in a Plane: Trigonometric identities for the strains: ' ' ε + ε 33 = ε + ε 33, ( ) = (ε ) + (ε ) ε ε 33 ( ε 3 ) = (ε1 ) + ( ε 13 ) ' ε ' 1 ' + ε 33 ' ε 3 ' 13, Form of W: W = W ε11, ε + ε 33, ε ε 33 ( ε 3 ), ( ε 1 ) + ( ε 13 ) ) ' ' ' ' ' ' ε 33 W = W ε 11, ε + ε 33, ε ε 3 ( ( ),( ) + ( ) ' ε1 ' ε13
39 Isotropy in a Plane: Strain energy density function for orthotropic material: W = C11ε 11 + C1 ε 11ε + C13ε 11ε 33 + C ε + C 33ε 33 + C 3ε ε C 44 ε 3 + 4C 55ε C 66 ε 1 rearranging W = C11ε 11 + ε 11 ( C1 ε + C13ε 33 ) + 4C55ε C 66 ε C 33ε 33 + C 3ε ε C 44 ε 3 + C ε
40 Isotropy in a Plane: W = C11ε 11 + ε 11 ( C1 ε + C13ε 33 ) + 4C55ε C 66 ε C ε + C 33ε 33 + C 3ε ε C 44 ε 3 In the second bracket, we take C1 = C13 In the third bracket, we take C55 = C 66 C = C33 and C 3 + C 33ε 33 + C 3ε ε C 44ε 3 Rearrange the last bracket with C ε unchanged = C ( ε + ε 33 ) C ε ε 33 + C 3ε ε C 44 ε 3
41 Isotropy in a Plane: Rearrange the last bracket further as C ε + C 33ε 33 + C 3ε ε C 44 ε 3 = C ( ε + ε 33 ) we need C 44 ( C C 3 ) ε ε 33 C 44 ε 3 C C 3 =
42 Isotropy in a Plane: Stiffness tensor C11 C ij = C1 C1 0 0 C C C 0 0 C C 3 0 Sym C 66 5 independent constants Such materials are called Transversely isotropic materials. Define: where C 66
43 Transverse Isotropy with an Additional Orthogonal Plane: Consider isotropy in x1x plane as well strain transformation
44 Transverse Isotropy with an Additional Orthogonal Plane: Trigonometric identities: ε 11 + ε = ' ε 11 ' + ε, ( ) = (ε ) + (ε ) ε 11ε ( ε 1 ) = (ε13 ) + ( ε 3 ) ' ε 11 ' + ε ' 13 ' ε 1 ' 3, Form of W: W = W ε11 + ε, ε 33, ε 11ε ( ε 1 ), ( ε13 ) + ( ε 3 ) ) ' ' ' ' ' ' ε ε1 W = W ε 11 + ε, ε 33, ε 11 ( ( ),( ) + ( ) ' ε13 ' ε 3
45 Transverse Isotropy with an Additional Orthogonal Plane: In the second bracket, we take C1 = C 3 In the third bracket, we take Rearrange the last bracket with C11 = C and C1 unchanged
46 Isotropy: Two independent constants! C11 Cij = C1 C1 0 0 C11 C1 0 0 C C11 C1 0 Define: where C11 C1 Sym C11 C1 0
47 3D Constitutive Relations: Quick Review Generalized Hooke s Law: 81 independent constants Stress tensor symmetry: 54 independent constants Strain tensor symmetry: 36 independent constants Existence of W (Hyperelastic/Aelotropic): 1 independent constants Existence of one plane of material symmetry: 13 independent constants Existence of two/three mutually perpendicular planes of symmetry: (Orthotropic Material) 9 independent constants One plane of isotropy: 5 independent constants Two/three/infinite planes of isotropy: independent constants
48 3D Constitutive Relations for Orthotropic Materials
49 Constitutive Relations for Orthotropic Materials: Strainstress Relations Normal stresses and strains
50 Constitutive Relations for Orthotropic Materials: Shear stresses and strains Poisson s ratio: (no sum over i, j) In general, ν ij ν ji
51 Constitutive Relations for Orthotropic Materials: Determination of Engineering Constants:
52 Constitutive Relations for Orthotropic Materials: Matrixvector form: where, Always work with compliance tensor. It is easy to remember.
53 Constitutive Relations for Orthotropic Materials: Important Relations: Reciprocal relation where,
54 Constitutive Relations for Orthotropic Materials: Stiffness Relations: where,
55 Constraints on Engineering Constants: For strain energy to be positive definite both Compliance and Stiffness tensors must be positive definite. Strain energy to be positive definite the diagonal entries of the Compliance tensor must be positive. Similarly, the diagonal entries of the Stiffness tensor must be positive and the determinant must also be positive
56 Constraints on Engineering Constants: Constraint on Poisson s ratio: From constraint on determinant:
57 Constraints on Engineering Constants: For transverse isotropic material: with we get, Finally, leads to the condition For isotropic materials: and
58 Constitutive Relations: Transformations 13 Principal material directions xyz global reference directions Transformation matrix for rotation about zaxis:
59 Constitutive Relations: Stress Transformations Stress transformation: ' σ ij For example, that is, Transformation matrix: = a ki aljσ kl
60 Constitutive Relations: Stress and Strain Transformations Transformation matrix: where, m=cosθ and n=sinθ
61 Constitutive Relations: Stress and Strain Transformations Stress transformation: ' ε ij For example, that is, Now using = a ki alj ε kl
62 Constitutive Relations: Stress and Strain Transformations Strain transformation: Transformation matrix:
63 Constitutive Relations: Stress and Strain Transformations Stress Transformation: Strain Transformation:
64 Constitutive Relations: Stiffness Transformations From the first principles: Writing in global coordinates leads to and
65 Constitutive Relations: Stiffness Transformations Results in monoclinic behaviour! Constitutive relations:
66 Constitutive Relations: Stiffness Transformations
67 Constitutive Relations: Compliance Transformations From the first principles: Writing in global coordinates Or and
68 Constitutive Relations: Compliance Transformations The transformed Stiffness and Compliance tensors are symmetric! From invariance of W one can show 1 [T1 ] T = [T ] and 1 [T ] T = [T1 ]
69 Constitutive Relations: Compliance Transformations
70 Constitutive Relations: Thermal Effects Coefficient of thermal expansion is different in 3 directions!
71 Constitutive Relations: Thermal Effects Thermal strain in principal material directions where, These strains will not produce stresses unless restricted! Transforming strains into global coordinates We get,
72 Constitutive Relations: Thermal Effects That is, where, and
73 Constitutive Relations: ThermoElastic Equations Total strains: Mechanical strains: Thus, gives the thermoelastic constitutive equations as
74 Constitutive Relations: ThermoElastic Equations Stresses in global direction: where,
75 Constitutive Relations: Hygral Effects Hygral strains: where, are coefficient s of hygral expansion
76 Constitutive Relations: HygroThermal Effects Total strains: with, The hygrothermoelastic constitutive equation:
77 D Constitutive Relations for Orthotropic Materials
78 Constitutive Relations: Planar Equations Constitutive relation in 3D: Transverse stresses are zero: σ zz = τ xz = τ yz = 0 γ yz = S 44τ yz + S 45τ xz = 0 leads to γ xz = S 45τ xz + S 55τ yz = 0
79 Constitutive Relations: Transverse Strain Transverse normal strain: ε zz = S 13σ xx + S 3σ yy + S 36τ xy 0
80 Constitutive Relations: InPlane Stresses
81 Constitutive Relations: InPlane Stresses
82 Constitutive Relations: Planar Equations Constitutive relation in 3D (Principal Directions): Transverse stresses are zero: leads to
83 Planar Relations: Principal Directions Transverse normal strain: ε 33 = S13σ 11 + S 3σ + S 36 τ 1 0 that is, ε 33 = S13σ 11 + S 3σ 0 Therefore, for planar case
84 Planar Relations: Principal Directions Transverse normal strain from stiffness relations: Transverse normal stress: gives
85 Planar Relations: Principal Directions Stresses in principal directions: Putting ε 33 in terms of ε 11, ε
86 Planar Relations: Principal Directions Stresses in principal directions: And can be written in a form as Qij and Cij are not same Inverse f orm: Sij are same as in 3D relations
87 Planar Relations: Principal Directions Reduced Stiffness Matrix: Stiffness Compliance in terms of engineering constants
88 Planar Relations: Principal Directions Stresses in principal directions:
89 Planar Relations: Principal Directions Stresses in principal directions:
90 Planar Relations: Transformation of Stresses and Strains Stresses in principal directions: Strains in principal directions:
91 Planar Relations: Transformation of Stresses and Strains Stresses in principal directions:
92 Planar Relations: Transformation of Stresses and Strains
93 Planar Relations: Transformation of Stresses and Strains Stresses in principal directions:
94 Planar Relations: Hygrothermoelastic Relations Stresses in principal directions: Stresses in principal directions Stresses in global directions:
95 Thank You
Understand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationConstitutive Relations
Constitutive Relations Dr. Andri Andriyana Centre de Mise en Forme des Matériaux, CEMEF UMR CNRS 7635 École des Mines de Paris, 06904 Sophia Antipolis, France Spring, 2008 Outline Outline 1 Review of field
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationConstitutive Relations
Constitutive Relations Andri Andriyana, Ph.D. Centre de Mise en Forme des Matériaux, CEMEF UMR CNRS 7635 École des Mines de Paris, 06904 Sophia Antipolis, France Spring, 2008 Outline Outline 1 Review of
More information16.21 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive Equations
6.2 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive quations Constitutive quations For elastic materials: If the relation is linear: Û σ ij = σ ij (ɛ) = ρ () ɛ ij σ ij =
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More information3.2 Hooke s law anisotropic elasticity Robert Hooke ( ) Most general relationship
3.2 Hooke s law anisotropic elasticity Robert Hooke (16351703) Most general relationship σ = C ε + C ε + C ε + C γ + C γ + C γ 11 12 yy 13 zz 14 xy 15 xz 16 yz σ = C ε + C ε + C ε + C γ + C γ + C γ yy
More informationModule 3: 3D Constitutive Equations Lecture 10: Constitutive Relations: Generally Anisotropy to Orthotropy. The Lecture Contains: Stress Symmetry
The Lecture Contains: Stress Symmetry Strain Symmetry Strain Energy Density Function Material Symmetry Symmetry with respect to a Plane Symmetry with respect to two Orthogonal Planes Homework References
More information2.2 Relation Between Mathematical & Engineering Constants Isotropic Materials Orthotropic Materials
Chapter : lastic Constitutive quations of a Laminate.0 Introduction quations of Motion Symmetric of Stresses Tensorial and ngineering Strains Symmetry of Constitutive quations. ThreeDimensional Constitutive
More informationPEAT SEISMOLOGY Lecture 2: Continuum mechanics
PEAT8002  SEISMOLOGY Lecture 2: Continuum mechanics Nick Rawlinson Research School of Earth Sciences Australian National University Strain Strain is the formal description of the change in shape of a
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More information16.20 HANDOUT #2 Fall, 2002 Review of General Elasticity
6.20 HANDOUT #2 Fall, 2002 Review of General Elasticity NOTATION REVIEW (e.g., for strain) Engineering Contracted Engineering Tensor Tensor ε x = ε = ε xx = ε ε y = ε 2 = ε yy = ε 22 ε z = ε 3 = ε zz =
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationChapter 2 General Anisotropic Elasticity
Chapter 2 General Anisotropic Elasticity Abstract This Chapter is an introduction to general anisotropic elasticity, i.e. to the elasticity of 3D anisotropic bodies. The main classical topics of the matter
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationMacroscopic theory Rock as 'elastic continuum'
Elasticity and Seismic Waves Macroscopic theory Rock as 'elastic continuum' Elastic body is deformed in response to stress Two types of deformation: Change in volume and shape Equations of motion Wave
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 24 Analysis of an Orthotropic Ply Lecture Overview Transformation of stresses and strains Stress
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationElasticity in two dimensions 1
Elasticity in two dimensions 1 Elasticity in two dimensions Chapters 3 and 4 of Mechanics of the Cell, as well as its Appendix D, contain selected results for the elastic behavior of materials in two and
More information1 Hooke s law, stiffness, and compliance
Nonquilibrium Continuum Physics TA session #5 TA: Yohai Bar Sinai 3.04.206 Linear elasticity I This TA session is the first of three at least, maybe more) in which we ll dive deep deep into linear elasticity
More informationTensor Visualization. CSC 7443: Scientific Information Visualization
Tensor Visualization Tensor data A tensor is a multivariate quantity Scalar is a tensor of rank zero s = s(x,y,z) Vector is a tensor of rank one v = (v x,v y,v z ) For a symmetric tensor of rank 2, its
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationA short review of continuum mechanics
A short review of continuum mechanics Professor Anette M. Karlsson, Department of Mechanical ngineering, UD September, 006 This is a short and arbitrary review of continuum mechanics. Most of this material
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More informationGG303 Lecture 6 8/27/09 1 SCALARS, VECTORS, AND TENSORS
GG303 Lecture 6 8/27/09 1 SCALARS, VECTORS, AND TENSORS I Main Topics A Why deal with tensors? B Order of scalars, vectors, and tensors C Linear transformation of scalars and vectors (and tensors) II Why
More informationNDT&E Methods: UT. VJ Technologies CAVITY INSPECTION. Nondestructive Testing & Evaluation TPU Lecture Course 2015/16.
CAVITY INSPECTION NDT&E Methods: UT VJ Technologies NDT&E Methods: UT 6. NDT&E: Introduction to Methods 6.1. Ultrasonic Testing: Basics of ElastoDynamics 6.2. Principles of Measurement 6.3. The PulseEcho
More informationStress/Strain. Outline. Lecture 1. Stress. Strain. Plane Stress and Plane Strain. Materials. ME EN 372 Andrew Ning
Stress/Strain Lecture 1 ME EN 372 Andrew Ning aning@byu.edu Outline Stress Strain Plane Stress and Plane Strain Materials otes and News [I had leftover time and so was also able to go through Section 3.1
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam
MODELING OF CONCRETE MATERIALS AND STRUCTURES Class Meeting #1: Fundamentals Kaspar Willam University of Colorado at Boulder Notation: Direct and indicial tensor formulations Fundamentals: Stress and Strain
More informationSymmetry and Properties of Crystals (MSE638) Stress and Strain Tensor
Symmetry and Properties of Crystals (MSE638) Stress and Strain Tensor Somnath Bhowmick Materials Science and Engineering, IIT Kanpur April 6, 2018 Tensile test and Hooke s Law Upto certain strain (0.75),
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationLearning Units of Module 3
Module Learning Units of Module M. tresstrain oncepts in Three Dimension M. Introduction to Anisotropic lasticity M. Tensorial oncept and Indicial Notations M.4 Plane tress oncept Action of force (F)
More informationUnit IV State of stress in Three Dimensions
Unit IV State of stress in Three Dimensions State of stress in Three Dimensions References Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationMechanics of Biomaterials
Mechanics of Biomaterials Lecture 7 Presented by Andrian Sue AMME498/998 Semester, 206 The University of Sydney Slide Mechanics Models The University of Sydney Slide 2 Last Week Using motion to find forces
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More information3.22 Mechanical Properties of Materials Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 3.22 Mechanical Properties of Materials Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Quiz #1 Example
More informationIntroduction to Seismology Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 12.510 Introduction to Seismology Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Stress and Strain
More informationCH.6. LINEAR ELASTICITY. Multimedia Course on Continuum Mechanics
CH.6. LINEAR ELASTICITY Multimedia Course on Continuum Mechanics Overview Hypothesis of the Linear Elasticity Theory Linear Elastic Constitutive Equation Generalized Hooke s Law Elastic Potential Isotropic
More informationVariational principles in mechanics
CHAPTER Variational principles in mechanics.1 Linear Elasticity n D Figure.1: A domain and its boundary = D [. Consider a domain Ω R 3 with its boundary = D [ of normal n (see Figure.1). The problem of
More informationA STUDY OF HYDRAULIC FRACTURE INITIATION IN TRANSVERSELY ISOTROPIC ROCKS. A Thesis VAHID SERAJIAN
A STUDY OF HYDRAULIC FRACTURE INITIATION IN TRANSVERSELY ISOTROPIC ROCKS A Thesis by VAHID SERAJIAN Submitted to the Office of Graduate Studies of Texas A&M University in partial fulfillment of the requirements
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationIntroduction, Basic Mechanics 2
Computational Biomechanics 18 Lecture : Introduction, Basic Mechanics Ulli Simon, Lucas Engelhardt, Martin Pietsch Scientific Computing Centre Ulm, UZWR Ulm University Contents Mechanical Basics Moment
More informationChapter 2. Rubber Elasticity:
Chapter. Rubber Elasticity: The mechanical behavior of a rubber band, at first glance, might appear to be Hookean in that strain is close to 100% recoverable. However, the stress strain curve for a rubber
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationGEOMETRIC NONLINEAR ANALYSIS
GEOMETRIC NONLINEAR ANALYSIS The approach for solving problems with geometric nonlinearity is presented. The ESAComp solution relies on Elmer opensource computational tool [1] for multiphysics problems.
More informationTensor Transformations and the Maximum Shear Stress. (Draft 1, 1/28/07)
Tensor Transformations and the Maximum Shear Stress (Draft 1, 1/28/07) Introduction The order of a tensor is the number of subscripts it has. For each subscript it is multiplied by a direction cosine array
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More information19. Principal Stresses
19. Principal Stresses I Main Topics A Cauchy s formula B Principal stresses (eigenvectors and eigenvalues) C Example 10/24/18 GG303 1 19. Principal Stresses hkp://hvo.wr.usgs.gov/kilauea/update/images.html
More informationThe Finite Element Method
The Finite Element Method 3D Problems Heat Transfer and Elasticity Read: Chapter 14 CONTENTS Finite element models of 3D Heat Transfer Finite element model of 3D Elasticity Typical 3D Finite Elements
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationUseful Formulae ( )
Appendix A Useful Formulae (985989993) 34 Jeremić et al. A.. CHAPTER SUMMARY AND HIGHLIGHTS page: 35 of 536 A. Chapter Summary and Highlights A. Stress and Strain This section reviews small deformation
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationProblem Set 2 Due Tuesday, September 27, ; p : 0. (b) Construct a representation using five d orbitals that sit on the origin as a basis: 1
Problem Set 2 Due Tuesday, September 27, 211 Problems from Carter: Chapter 2: 2ad,g,h,j 2.6, 2.9; Chapter 3: 1ad,f,g 3.3, 3.6, 3.7 Additional problems: (1) Consider the D 4 point group and use a coordinate
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Overview Milestones in continuum mechanics Concepts of modulus and stiffness. Stressstrain relations Elasticity Surface and body
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationPart 5 ACOUSTIC WAVE PROPAGATION IN ANISOTROPIC MEDIA
Part 5 ACOUSTIC WAVE PROPAGATION IN ANISOTROPIC MEDIA Review of Fundamentals displacementstrain relation stressstrain relation balance of momentum (deformation) (constitutive equation) (Newton's Law)
More informationMICROMECHANICS AND HOMOGENIZATION. Materials Containing Coated and Uncoated Spherical Inhomogeneities
MICROMECHANICS AND HOMOGENIZATION Materials Containing Coated and Uncoated Spherical Inhomogeneities Václav Nežerka, 2012 i Acknowledgement I would like to thank my supervisor, Jan Zeman, who supported
More informationSolid State Theory Physics 545
olid tate Theory hysics 545 Mechanical properties of materials. Basics. tress and strain. Basic definitions. Normal and hear stresses. Elastic constants. tress tensor. Young modulus. rystal symmetry and
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationIntroduction to Seismology Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 1.510 Introduction to Seismology Spring 008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. 1.510 Introduction to
More informationConstitutive models: Incremental (Hypoelastic) Stress Strain relations. and
Constitutive models: Incremental (Hypoelastic) Stress Strain relations Example 5: an incremental relation based on hyperelasticity strain energy density function and 14.11.2007 1 Constitutive models:
More information1 Stress and Strain. Introduction
1 Stress and Strain Introduction This book is concerned with the mechanical behavior of materials. The term mechanical behavior refers to the response of materials to forces. Under load, a material may
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationContinuum Mechanics Fundamentals
Continuum Mechanics Fundamentals James R. Rice, notes for ES 220, 12 November 2009; corrections 9 December 2009 Conserved Quantities Let a conseved quantity have amount F per unit volume. Examples are
More informationOn commutativity of Backus and Gazis averages
On commutativity of ackus and Gazis averages David R. Dalton Michael A. Slawinski arxiv:1601.0969v1 [physics.geoph] 1 Jan 016 Abstract January 1 016 We show that the ackus (196 equivalentmedium average
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More informationClassical Mechanics. Luis Anchordoqui
1 Rigid Body Motion Inertia Tensor Rotational Kinetic Energy Principal Axes of Rotation Steiner s Theorem Euler s Equations for a Rigid Body Eulerian Angles Review of Fundamental Equations 2 Rigid body
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationEngineering Sciences 241 Advanced Elasticity, Spring Distributed Thursday 8 February.
Engineering Sciences 241 Advanced Elasticity, Spring 2001 J. R. Rice Homework Problems / Class Notes Mechanics of finite deformation (list of references at end) Distributed Thursday 8 February. Problems
More informationProperties of the stress tensor
Appendix C Properties of the stress tensor Some of the basic properties of the stress tensor and traction vector are reviewed in the following. C.1 The traction vector Let us assume that the state of stress
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationOn the stressbased and strainbased methods for predicting optimal orientation of orthotropic materials
Research paper Struct Multidisc Optim 6, 9 34 004 DOI 10.1007/s001580030348x On the stressbased and strainbased methods for predicting optimal orientation of orthotropic materials H.C. Gea, J.H. Luo
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationDepartment of Mechanical Engineering, National Institute of Technology Rourkela, Rourkela , India
Composites, Article ID 629175, 12 pages http://dx.doi.org/10.1155/2014/629175 Research Article Effect of Fiber Geometry and Representative Volume Element on Elastic and Thermal Properties of Unidirectional
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationABHELSINKI UNIVERSITY OF TECHNOLOGY
ABHELSINKI UNIVERSITY OF TECHNOLOGY TECHNISCHE UNIVERSITÄT HELSINKI UNIVERSITE DE TECHNOLOGIE D HELSINKI A posteriori error analysis for the Morley plate element Jarkko Niiranen Department of Structural
More informationChapter 5 PlaneStress StressStrain Relations in a Global Coordinate System
Chapter 5 PlaneStress StressStrain Relations in a Global Coordinate System One of the most important characteristics of structures made of fiberreinforced materials, and one which dictates the manner
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More information